Formation of a nanometer-thick water layer at high humidity on a dynamic crystalline material composed of multi-interactive molecules
Yumi Yakiyama; Gil Ryeong Lee; Sung Yeon Kim; Yoshitaka Matsushita; Yasushi Morita; Moon Jeong Park; Masaki Kawano; Chem.Commun. 51 (2015) 6828–; doi:10.1039/C5cc01568E

data_7116943
_publ_section_title
;
 Formation of a nanometer-thick water layer at high humidity on a dynamic
 crystalline material composed of multi-interactive molecules
;
_journal_name_full               Chem.Commun.
_journal_page_first              6828
_journal_paper_doi               10.1039/C5cc01568E
_journal_volume                  51
_journal_year                    2015
_chemical_formula_sum            'C22 K N9 O2'
_chemical_formula_weight         460.98
_chemical_name_systematic        ' ?'
_space_group_crystal_system      monoclinic
_space_group_IT_number           13
_space_group_name_H-M_alt        'P 1 2/a 1'
_symmetry_Int_Tables_number      13
_symmetry_space_group_name_Hall  '-P 2ya'
_symmetry_space_group_name_H-M   'P 1 2/a 1'
_audit_update_record
;
2014-10-25 deposited with the CCDC.
2015-03-19 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 104.65(3)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   20.904(11)
_cell_length_b                   15.931(10)
_cell_length_c                   9.711(5)
_cell_measurement_temperature    298
_cell_volume                     3129(3)
_computing_cell_refinement       'RIETAN-FP (Izumi and Momma, 2007)'
_computing_data_collection       'DIFFRAC plus'
_computing_molecular_graphics    'VESTA (Momma and Izumi, 2008)'
_computing_structure_refinement  'RIETAN-FP (Izumi and Momma, 2007)'
_computing_structure_solution    DASH
_diffrn_ambient_temperature      298
_diffrn_detector                 Scintillation
_diffrn_detector_type            LynxEye
_diffrn_measurement_device_type  'D8 ADVANCE'
_diffrn_radiation_monochromator  'Ge 111'
_diffrn_radiation_type           'Cu K_alpha radiation'
_diffrn_radiation_wavelength     1.5406
_diffrn_source                   Conventional
_diffrn_source_target            Cu
_diffrn_source_type              'Sealed tube'
_pd_block_diffractogram_id       '1 d-dried_3'
_pd_char_colour                  'pale yellow'
_pd_instr_location               ' ?'
_pd_meas_2theta_range_inc        0.0184
_pd_meas_2theta_range_max        49.9971
_pd_meas_2theta_range_min        3.0000
_pd_meas_number_of_points        2555
_pd_meas_scan_method             step
_pd_proc_info_excluded_regions   49.4446-49.9971
_pd_proc_ls_background_function  'Refine background parameters'
_pd_proc_ls_pref_orient_corr     ' ?'
_pd_proc_ls_profile_function     'Modified split pseudo-Voigt function'
_pd_proc_ls_prof_R_factor        0.03043
_pd_proc_ls_prof_wR_expected     0.07351
_pd_proc_ls_prof_wR_factor       0.04847
_pd_spec_mounting                ' ?'
_pd_spec_mount_mode              reflection
_pd_spec_shape                   flat_sheet
_pd_spec_size_axial              20
_pd_spec_size_equat              20
_pd_spec_size_thick              0.5
_refine_ls_goodness_of_fit_all   0.6594
_refine_ls_matrix_type           full
_refine_ls_number_constraints    0
_refine_ls_number_parameters     185
_refine_ls_number_restraints     160
_refine_ls_R_factor_all          0.01443
_refine_ls_R_Fsqd_factor         0.00953
_refine_ls_R_I_factor            0.01002
_refine_ls_shift/su_max          1.0E-6
_refine_ls_weighting_scheme      sigma
_cod_data_source_file            c5cc01568e2.cif
_cod_data_source_block           1_day-dried_KTPHAP_powder_3
_cod_original_cell_volume        3128(3)
_cod_original_sg_symbol_H-M      'P 2/a'
_cod_original_formula_sum        'C22 N9 O2 K1'
_cod_database_code               7116943